Ingeniare. Revista Chilena de Ingeniera
Universidad de Tarapac
Ponce L., Ernesto; de la Vega, Jos
Restoration of ancient bronze bells. Part I: powder metallurgy
Ingeniare. Revista Chilena de Ingeniera, vol. 22, nm. 4, octubre, 2014, pp. 460-468
Universidad de Tarapac
Available in: http://www.redalyc.org/articulo.oa?id=77231865002
How to cite
More information about this article
Journal's homepage in redalyc.org
Scientific Information System
Network of Scientific Journals from Latin America, the Caribbean, Spain and Portugal
Non-profit academic project, developed under the open access initiative
Ingeniare. Revista chilena de ingeniera, vol.22 N4, 2014, pp.460-468
Restoration of ancient bronze bells. Part I: powder metallurgy
Restauracin de antiguas campanas de bronce. Parte I: pulvimetalurgia
Ernesto Ponce L.1 Jos de la Vega1
Recibido 17 de abril de 2014, aceptado 25 de junio de 2014Received: April 17, 2014 Accepted: June 25, 2014
There is a big number of church bells from the Colonial Period in the highlands of Northern Chile, which are damaged by use during centuries and by falls due to earthquakes that periodically affect the region. The aim of this work was to create a non-invasive method to restore these valuable pieces, leaving minimum trace of repair. A fissured church bell from the late nineteenth century was restored. Powder metallurgy was used to repair only in the thin line of the crack, and to prevent coarse material removal action on both sides of the crack, with subsequent filling with conventional weld at high temperatures. Fissures were filled with copper and tin powder, which were then welded with tin at a low temperature. The advantage of this method is that it does not cause local heating that can brittle the vicinity of the welded area, resulting in a smooth joint and a good adhesion surface for good sound transmission that can withstand stresses. Results: In order to verify the efficiency of the method, joint material strength was measured, and the sound was compared to the dominant note required by the DIN4178 Standard. A finite element model incorporating a filler ring in the repair area was as well verified. The rationale for these repair works lies in that the old bells in question need to be preserved, since they are culturally valuable artifacts that hold rich metallurgical knowledge and are part of the national heritage.
Keywords: Metallurgy restoration, powder metallurgy, ancient metallurgy, bells, bronze welding, finite elements, crack repair.
Existe una gran cantidad de campanas del perodo colonial pertenecientes a iglesias del Altiplano del Norte chileno, que se encuentran daadas por el uso durante siglos y por cadas debido a los sismos que peridicamente afectan la regin. El objetivo fue crear un mtodo no invasivo para restaurar estas valiosas piezas, dejando un mnimo rastro de la reparacin. Se restaur una campana de iglesia de fines del siglo XIX que estaba agrietada. Se emple metalurgia de polvos para reparar solo en la delgada lnea de la fisura y evitar la invasiva accin de extraer material en ambos lados de la grieta, con el posterior relleno con soldaduras convencionales a temperaturas mayores. Se rellenaron las fisuras con cobre y estao en polvo que luego se sold con estao, a baja temperatura. Las ventajas del mtodo radican en no producir un calentamiento local que fragilice la vecindad de la soldadura, dar una unin de superficie lisa de gran adherencia que da una buena transmisin del sonido y capaz de soportar tensiones. Resultados: Para comprobar su eficiencia se midi la resistencia del material de la unin, tambin se compar el sonido con la nota dominante que debi tener la campana segn Norma DIN 4178. Otra verificacin fue un modelo de elementos finitos que incorpora un anillo de material de aporte en el sector de la reparacin. Se justifican estos trabajos porque las campanas necesitan ser conservadas, ya que encierran una gran riqueza cultural y conocimientos metalrgicos que son patrimonio de la nacin.
Palabras clave: Restauracin metalrgica, pulvimetalurgia, metalurgia antigua, campanas, soldadura para bronce, elementos finitos, reparacin de grietas.
1 Escuela Universitaria de Ingeniera Mecnica. Universidad de Tarapac. Casilla 6-D. Arica, Chile. E-mail: [email protected]; [email protected]
Ponce L. and De la Vega: Restoration of ancient bronze bells. Part I: powder metallurgy
In order to convert the colonies in the Americas into Catholicism, a big number of churches were erected since the end of the 16th century. This occurred as well in the highlands and foothills in the northernmost part Chile. Many colonial churches and bells can still be found in this area. They have survived use and earthquakes for centuries. The architecture by then was a combination of Spanish 16th-17th century style and local materials and indigenous labor. In Northern Chile, indigenous peoples still appreciate their churches and bell towers, since they are integral part of the local culture. Churches and their bell towers were once part of their lives, with religious festivals, processions and rites still happening there. Bells were very important to call for the parishioners to come to celebrations and to mass. According to the Catholic tradition, the size of bells was in accordance with the number of inhabitants in a village or town; e.g. for a 5,000 inhabitant town, a bell required to have a weight of approximately 1,000 kg . Each tower bell had more than one bell, a big one and other small ones that were used for everyday services.
Casting techniques were based on European technologies, but there were not fixed patterns for geometry, except in some cases. They were placed in a mold with a clay and sand mix (some remains can still be found to be attached to the bell bends). The mold consisted of an internal nucleus made in a horizontal lathe, and an external layer. An empty space was left between the two molds. The axis of the bell was kept in vertical position on a horizontal platform made of abode and mortar. Molten metal was poured from an upper open through on the external mold. On the upper part, below the open trough, there were handles to hold the finished piece in the bell tower. The open trough allowed for the metal to contract while solidifying, without affecting the handles. In most of the pieces under study, the wall thickness is greater than that of European bells, but external dimensions are similar.
The main smelter would not engrave his name on the bell, but did engrave the casting date and some other inscriptions in some exceptional cases. Some finishes were neither classic nor done by chisellers, which shows that the bells were built by local smelters. However, many of the bells show no cracks,
which is evidence of their creators knowledge of metallurgy. It is worth noting that a European bell is estimated to last for half a century, whereas bells found in the highlands have already had a life of over four centuries. No information is available on the smelters or those who financed the works.
Common alloys of the time contained approximately 78% copper and 22% tin. The use of lead and zinc was avoided because it affected the quality of sound. Nevertheless, old literature indicates a weight ratio as follows: 79 parts of copper, 23 parts of tin, and 6 parts of zinc, totalling 108 parts. Other smelters were more conservative and included only 2% zinc, with 78% copper and 20% tin. Zinc was called Indian tin and became known in Europe after the 12th century. At the beginning of the 12th century, it was proved that gold and silver did not improve the quality of sound, contrary to the thought of the time. These noble metals have not been detected in analyses of ancient bell bronze. It could have possibly been a smelters resort to keep the precious metal for themselves, since it was difficult to carry out reliable metallurgy analysis by that time.
Cracks on the bell walls were caused by the strikes of the clapper, which create compression waves that expand through the metal. In the wall thickness considered, when reaching the opposite surface, waves are reflected inverted as traction waves . Non-centrifuged old bronze withstands compression better than stress, because it is a more fragile material. This is why the crack starts near the external surface of the bell, even though the clapper has struck the inside wall. When vibrations are produced by strikes, the material is submitted to cyclic loads that cause material fatigue. Once a crack has occurred, it grows rapidly because stresses at the bottom of the fissure are proportional to the inverse of the square of its bend radius. The smaller the radius is, the higher the stresses at that point are. For a homogenous, impurity-free piece of material with no residual stresses, the stresses under the area of clapper strike are (for a conventional circular-arc profile church bell): parallel to the axis of the bell = 11.014 P, transverse to the bell axis = 4.333 P, P being the impact stress. This formulation resulted from , and geometry was obtained from . This suggests that longitudinal fissures prevail but not in all cases. When a bell is smelted and poured from its upper part at a low flow speed, smelting layers that cool down at different